microfabricated dry adhesive displaying frictional microfabricated dry adhesive displaying...
Post on 14-Jul-2020
Embed Size (px)
Microfabricated Dry Adhesive Displaying Frictional Adhesion
Daniel Soto, Aaron Parness, Noé Esparza, Tom Kenny, Kellar Autumn, Mark Cutkosky
3 jan 2008
We present in this abstract the fabrication and testing of an anisotropic dry adhesive that exhibits frictional adhesion, a behavior observed in the geckos’ adhesive. We have taken inspiration from the architectural principles of the gecko’s adhesive to create an anisotropic artificial adhesive from PDMS. This adhesive is created by a molding process that utilizes SU-8 as the mold material and PDMS as the cast material. By using an angled two-sided exposure process on a transparent substrate, we are able to create an asymmetrical structure of microwedges (Figure 1). This arrayed microstructure exhibits frictional adhesion. That is, its capacity to adhere to surfaces is described by a model unlike the familiar embedded friction cone models (Figure 4) exhibited by pressure sensitive adhesives such as tape or Post-it R© Notes. We have only previously observed this model in the gecko.
The mold is created by a dual sided lithography of SU-8 on a transparent substrate. The process flow is depicted in Figure 5. An aluminum masking layer is deposited and patterned followed by layer of SU-8. The wafer is placed on a tilting stage and is flood illuminated by UV light. A mask is aligned to the front side and another exposure is performed. After develop, the SU-8 has an array triangular pits. We cast and spin PDMS in the mold, yielding a flat backing layer with wedged tips protruding from the surface. We believe this process to be novel and of use to other researchers.
Once fabricated, we test the microwedge adhesive on a force testing apparatus with three axis motors to control friction and loading. An adhesive patch of ∼1cm2 is affixed to a load cell. A flat glass slide is brought into compressive contact and then pulled at a given angle. We collect data for both shear force and normal force adhesion during the period of contact. We perform the familiar load-drag-pull test that mimics the geckos adhesion mode. A more detailed test with multiple exit angles allows for the mapping out of a limit surface curve for the adhesive. The force trace plot (Figure 6) allows us to see the forces exerted by the adhesive as a function of time. As we see in Figure 6, dynamic sliding adhesion is obtained. The adhesive is able to simultaneously maintain 0.4 N/cm2 of adhesion and 2.0 N/cm2 of shear. We have not seen another adhesive that displays this dynamic adhesion property that the gecko displays. This property allows the microwedge adhesive a graceful failure mode desirable for robotics or locomotion applications. The force space plot (Figure 7) parameterizes the force trace plot using time and allows us to see the path through force space. The higher density of points in the lower left represents the dynamic sliding adhesion in another way. Lastly, the limit surface (Figure 9), obtained through many trials over a range of preload angles, preload depths, and exit angles, is a map of the release points for different shear to adhesion ratios. If we observe the limit surface (Figure 9), we see that the sample increases its adhesive strength as it is put into shear. If we compare this limit surface to that of a flat control (Figure 10), we see that it is different than the embedded friction cone model. We have also performed repeated testing of the adhesive over as many as 30,000 cycles. When loaded to a constant displacement depth, the microwedges retain 50% of their adhesion and 86% of their shear over the 30,000 trials. This is in contrast to conventional pressure sensitive adhesives which degrade quickly with repeated use.
We believe that this adhesive is an important advancement in applications where shear force, anisotropy, and reusability are key properties.
 K. Autumn, A. Dittmore, D. Santos, M. Spenko, and et al. Frictional adhesion: a new angle on gecko attachment. Journal of Experimental Biology, Jan 2006.
P70-50s: fibers appear to be relatively triangular with a thick base.
SYL170-50s: In comparison the base of this sample is much thinner, and the fibers have an hourglass shape
P20-50s: Base thickness is similar to that of P70 material, but the fibers are much more deformed and matted
SEM images: Side view
Figure 1: SEM Image of 50 µm Microwedges. Struc- tures are 50 µm square at the base and are 200 µm tall.
3571Frictional adhesion in gecko setae
maximum peeling force, which occurs at low angles, is limited by:
showing that stiffer materials, given the same adhesion energy, will peel at higher loads.
Peeling mechanics can apply – at least in theory – to fibrillar gecko-like materials (Hui et al., 2004). However, in real geckos where attachment is via a series of scansors bearing anisotropic setae, the validity of conventional (Kendall, 1975) peeling mechanics is less clear. Geckos hold their toes in a hyperextended position when not climbing – possibly protecting the scansors from abrasion (Russell, 1975), suggesting that DH could have functions other than reduction of detachment force via peeling mechanics. Indeed, it has been suggested that spatulae could detach more or less simultaneously (Gay, 2002), due to their mechanical independence. We tested the hypothesis of gecko pad detachment via peeling mechanics experimentally by measuring detachment angles of isolated setal arrays and live gecko toes, and evaluated the predictions of contact mechanical models of peeling using a computer simulation.
Materials and methods Live geckos
Tokay geckos (Gekko gecko L.) are capable of supporting many times their body weight by a single toe. We discovered that the normally aggressive and temperamental tokays became docile when attached by a single toe to a glass surface. Using a goniometer stage (Newport, Irvine, CA, USA), we slowly (
Shear stress (kPa)
'P20-50S 'P70-50s 'SYL170-50s 'P20-20s 'P70-20s 'SYL170-20s
Forwards LDP (SYL170-50s at 80μm preload)
Backwards LDP (SYL170-50s at 80μm preload)
Figure 6: Microwedge Force Trace. The normal trace shows the initial compression phase followed by a re- gion of adhesion during the parallel drag. In the shear trace, we see that there is a shear force created by the adhesive at the same time as the normal adhesion force.
−0.5 0 0.5 1 1.5 2 2.5 −0.5
Figure 7: Microwedge Force Space. This plot repre- sents data similar to that shown in Figure 6 but as a parametric plot. The plot begins at the origin and moves up the y-axis during the preload phase. As the sample is dragged the line moves into the fourth quadrant and lingers before returning to the origin.
3573Frictional adhesion in gecko setae
typical coefficient of friction of 0.31±0.02 (Fig.·3A,C), consistent with prior results (Autumn et al., 2006b).
Frictional adhesion When dragged along their natural curvature, isolated setal
arrays of geckos exhibit a very different tribological response than that predicted by previous friction/adhesion models or the Kendall tape peeling model (Eqn·1). As an array of setae began to slide along the surface, adhesion developed and persisted (Fig.·3B,D). Surprisingly, the ratio of shear force to adhesive force was approx. 2:1, irrespective of force magnitude
(Fig.·4A). To test the generality of this effect, we measured the angle at detachment ( *) in live geckos hanging by a single toe. The angle at which toes detach was 25.5±0.2° (N=181), similar to *=24.6±0.9° for isolated arrays. The peeling model predicts that larger forces cause lower values of * (see Eqn.·2). Instead, gecko toes detached at a constant angle regardless of applied force. These results are consistent with the function of single isolated setae (Autumn et al., 2000), which detach at an angle of 30.0±0.27° (Fig.·4B). Indeed, it is likely that the value of *=30° in single setae sets the upper limit for * at the array and toe levels.
Fig.·3. Shear and normal forces in isolated gecko setal arrays on a glass surface. Motion in normal and shear axes was controlled at 50· m·s–1. (A) Setal array during load (1), drag (2) and pull (3) (LDP) against the curvature of the setal shafts exhibits Coulomb friction. Negative F|| represents the reaction forces during a drag to the left. However, no difference between static and kinetic friction was evident. Compression force F was approx. 3.2 times shear force F||. (B) Setal array during LDP with the curvature of the setal shafts compressed initially, and then was pulled into tension as the setal tips adhered. Positive F|| represents the reaction forces during a drag to the right. Adhesion was sustained during the 100· m drag step (2). (C) Normal vs shear force during LDP against curvature of the setal shafts. F and F|| followed a path along the Coulomb friction cone (red broken line of slo